# MAGNETIC PROPERTIES OF Ni MnGa ALLOY

date post

09-Feb-2022Category

## Documents

view

0download

0

Embed Size (px)

### Transcript of MAGNETIC PROPERTIES OF Ni MnGa ALLOY

UntitledEvery spin-orbital ),,,,( 1 Mn RRr r

L rr σ from (13) can be represented as the product of spatial

orbital ),,,( 1 Mn RRr r

L rrψ and one of two spin functions )(σα or )(σβ corresponding to two

possible spin projection values of an electron. Expectation value of the electronic Hamiltonian eH N in LΦ state can be represented as

LL

( ) ,),,(),,( 2

1 ),,(),,(

r L

rr L

rr L

rr L

r (15)

where one-electron energies iE , Coulomb integrals ijJ and exchange integrals ijK all are

non-negative and defined as follows:

),,,,( 2

Obviously iiii KJ = .

Equations (16)-(18) show that for a fixed set of spin-orbitals contributing to

)RRr,r( MLLL

r L

rr L

r ,,,,,, 111 σσΦ the most adequate choose of the effective potential )(ri

r u

−= (19)

∑∫ ⋅ −

(21)

Such defined potential is named Hartree-Fock potential, it is non-local and depends on the spin-orbitals. The Koopman's theorem provides a physical interpretation of the orbital energies: it states that the orbital energy iε is an approximation of the ionization energy

associated with the removal of an electron from the orbital i .

Because of orbital dependence of Hartree-Fock potential, the orbitals themselves must be defined in a self-consistent manner. A trial set of spin-orbitals is formulated and used to

Magnetic properties of Ni2MnGa alloy 57

construct the Fock operator (11), where (18) is used for )(ri

r u , then the equations (12) are

solved to obtain a new set of spin-orbitals that are used to construct a revised Fock operator, and so on. The cycle of calculation and reformulation is repeated until a convergence criterion is satisfied. Such obtained spin-orbitals realize stationary point of energy (15) as functional of spin-orbitals (the latter are assumed to be orthonormal). In self-consistent field calculations on closed-shell states of atomic clusters with even number of electrons, it is supposed that the spatial parts of the spin-orbitals are identical for electrons of every electron pair. There are then L/2 spatial orbitals of the form

),,,( 1 Mn RRr r

.

)(),,,()(),,,(

)(),,,()(),,,(

)(),,,()(),,,(

)(),,,()(),,,(

rr

rrrr

(22)

.

)(),,,()(),,,(

)(),,,()(),,,(

)(),,,()(),,,(

)(),,,()(),,,(

)(),,,()(),,,(

rr

rrrr

(23)

In the unrestricted open-shell Hartree-Fock (UHF) formalism any two electrons are not constrained to the same spatial wave function and L-electron wave function has the general form (13). By relaxing the constraint of occupying orbitals in pairs, the open-shell UHF formalism gives a lower variational energy than the ROHF formalism. However, one disadvantage of the UHF approach is that whereas the RHF and ROHF wave functions are the eigenfunctions of the total cluster spin operator, the UHF function is not; that is, the total spin angular momentum is not well-defined for the UHF wavefunction. In practical calculations cluster spatial orbitals are expanded into a finite series of LK ≥

basis functions ),,( 1 Mk RRr r

L rrξ :

rr ξψ . (24)

It is useful to introduce vector and matrix notation for orbitals .}{};,,{};,,{ 11 kiKL C=== Cξψ ξξψψ LL (25)

Then, equation (24) can be rewritten as Cξψ = . (26)

T. Breczko, V.V. Barkaline, R.M. Grechishkin, V.V. Nelayev58

Then for closed shell RHF formalism energy relation (15) can be transformed to

,)} 2

r L

r (27)

If one introduces overlap matrix for the basis set orbitals

),,,(),,,( 11 MjMiij RRrRRrrd r

L rrr ξξ∫=S , the necessary and sufficient condition of

orthonormality for cluster orbitals can be represented as RRSR = . (31)

The stationarity condition for Hartree-Fock energy (27) accounting the orthonormality of the orbitals leads to Hartree-Fock matrix equations

SCεCGh =+ )( , (32) where ε is LL× matrix of Lagrange multipliers which can be chosen as a diagonal matrix with elements associated with the energies of corresponding cluster orbital. Similarly can be treated the case of open shells, with some sophistication of definition of G and C matrixes.

Density functional theory. An alternative to the HF methods is the density functional theory (DFT). DFT begins not with the multi-electron wavefunction

)RRr,r( MLL

r L

rr L

r ,,,,, 111 σσΦ and Schrödinger equation (7) but with the concept of the

electron probability density, which is defined as the integral over the spin coordinates of all electrons and over all but one of the spatial variables

)RRr,r()RRr,r(rdrdL

r

MLLMLLL

L

∑∫ ∫ (33)

This function determines the probability of finding any of the L electrons within a volume element rd

r . The reason for the popularity of DFT is that it takes into account electron

correlation. It can be used to do calculations on clusters of 100 or more atoms in significantly less time than HF methods. Integration of )(r

rρ over whole space gives the number of electrons in a cluster:

∫ = Lrrd )( rrρ . (34)

Major points of DFT theory is two Hohenberg-Kohn theorems. The first one demonstrates that the electron density uniquely determines the Hamiltonian operator and thus all the properties of the system. This theorem states that the external potential )(rN

r eV is (to

within a constant) a unique functional of )(r rρ . Since, in its turn )(rN

r eV fixes eH N , we see

Magnetic properties of Ni2MnGa alloy 59

that the full many particle ground state is a unique functional of )(r rρ . Thus, )(r

rρ

determines L and )(rN

r eV and hence all the properties of the ground state, for example the

kinetic energy ][ ρT , the potential energy of electron-nuclei interaction ][ ρeNV , the potential

energy of electron-electron interactions ][ ρeeV and the total electron energy ][ ρeNE , which

can be written as

,][)()(][][][][ ρρρρρρ HKNNN FrrrdVVTE +=++= ∫ rrr

eeeee V (35)

][][][ ρρρ eeVTFHK += . (36)

The second Hohenberg-Kohn theorem states that the functional ][ ρHKF , that delivers the ground state energy of the system, delivers the lowest energy if and only if the input density is the true ground state density. In other words this means that for any trial density )(~ r

rρ ,

which satisfies the necessary boundary conditions such as 0)(~ ≥r rρ , Lrrd =∫ )(~ rrρ , and

which is associated with some external potential )(rN

r eV , the energy obtained from functional

(35) represents an upper bound to the true ground state energy 0E . 0E results if and only if

the exact ground state density )(r rρ is inserted in (35).

From ][ ρeeV one can extract classical part ][ ρJ ,

][][][)()( 2

e rdrdV +=+

correction, exchange and Coulomb correlation. The explicit form of the functionals ][ ρT and ][ ρnclV is the major task of DFT. To relate

them to the well-known results of Hartree-Fock orbital theory the reference system of L non- interacting electrons with the same electron density function is introduced, for which the set of orthonormal spatial orbitals { } Liri ,,1,)( L

r =ψ defines

rhrr (39)

Then if one combines all unknown contributions into one energy term ][ ρXCE ,

,])[][(])[][(][ ρρρρρ JVTTE refXC −+−= ee (40)

the functional of cluster energy can be represented as

.][)()( 2 1

ee

(41)

The only term for which no explicit form can be given is ][ ρXCE . One now can apply the

variational principle to answer the question about what condition must the orbitals )(ri

rψ

fulfill in order to minimize the energy expression (41) under the usual constraint

ijji rrrd δψψ =∫ )()( rrr

,)()()( 2

ρ (43)

and δρρδ ][)( XCXC ErV =r is the variational derivative of exchange and correlation energy

functional. The value of )(rVKS

r depends on the density, and therefore the Kohn-Sham

equations have to be solved iteratively to obtain a self-consistent solution. Most of the applications of the Kohn-Sham density functional theory make use of the linear combination of atomic orbitals (LCAO) expansion of the Kohn-Sham orbitals. Similarly to (24), in this approach one introduces a set of K predefined basis functions

)(rk

∑ =

)()( rr ξψ . (44)

Basis functions for both SCF and DFT calculation usually are chosen among three possibilities:

I. Slater-type-orbitals (STO): they seem to be the natural choice for basis functions. They are exponential functions that mimic the exact eigenfunctions of a hydrogen atom. A typical STO is expressed as

),(1 θξ β lm

rnSTO YerN −−= . (45)

Here n corresponds to the principal quantum number, the orbital exponent is termed β and ),( θlmY are the usual spherical harmonics. Unfortunately, it is very difficult to

compute many-center integrals with STO basis, and they do not play a major role in ordinary quantum chemistry. II. Gaussian-type-orbitals (GTO). They have the following general form:

. 2rnmlGTO ezyxN αξ −= (46)

N is a normalization factor, α represents the orbital exponent. nmlJ ++= is used to classify the GTO as s-functions ( 0=J ), p-functions ( 1=J ), etc. III. Contracted Gaussian functions (CGF) basis sets, in which several Gaussian functions are combined in a fixed linear combination:

. 1

= = (47)

A variety of exchange-correlation functionals, having names such as mPWPW91, B3LYP, MPW1K, PBE1PBE, BLYP, BP91, and PBE, have been developed for use in DFT calculations; the names designate a particular pairing of an exchange functional and a correlation functional. For example, BLYP functional is a combination of the gradient- corrected exchange functional developed by A.D. Becke and the gradient-corrected correlation functional developed by C. Lee, W. Yang, and R.G. Parr. Some of the functionals, such as B3LYP, represent hybrid DFT calculations that use Hartree-Fock corrections in conjunction with density functional correlation and exchange Density functional theory has also been applied to study open-shell atoms and molecules on the basis of spin density concept. The spin density refers to the difference between the spin-up electron density and the spin-down electron density, and the exchange-correlation energy depends on the spin density as well as the total electron density. Namely such

Magnetic properties of Ni2MnGa alloy 61

approach has to be used in DFT investigations of the magnetic structures of metals and alloys. The original density functional theory has been generalized to deal with many different situations: spin polarized systems, multicomponent systems such as nuclei and electron hole droplets, free energy at finite temperatures, superconductors with electronic pairing mechanisms, relativistic electrons, time-dependent phenomena and excited states, bosons, molecular dynamics, etc. The computation time required for a DFT calculation formally scales as the third power of the number of basis functions; as a result, DFT methods are computationally more efficient (though not necessarily more accurate) than HF-based formalisms, which scale as the fourth power of the number of basis functions. 4. Computer simulations results and discussion Ni2MnGa Heusler alloys (HA) has a theoretical lattice constant of 5.811 Å (10.981 .u.) and 5.729 Å (10.826 .u.) for the ferromagnetic and the paramagnetic phase, respectively. The crystal structure of Ni2MnGa HA can be considered as a bcc-based fcc crystal with a chain of Ni-Mn-Ni-Ga along the <111> direction. In present paper simulations deal with the simplest structure unit of the material – the cluster containing 9 atoms which is presented in Fig. 2. We calculate electronic structure of this cluster by open shell restricted Hartree-Fock method (ROHF), by unrestricted Hartree-Fock method and density functional theory (DFT) using NWChem package [11]1. All calculations deal with the system of 252 electrons.

Fig. 2. Atomic structure of cluster NiMn4Ga4, the constitutive element of L21 cubic form of

Ni2MnGa. Basis sets used in calculations are presented in Table 3. In all cases 6-31G* was used to represent atomic orbitals of Ni and Mn, and 6-311G** for Ga atoms in ROHF calculations. For DFT calculations the simplest 3-21G basis set for Ga was used. Contracted Gaussian functions (47) are used to represent atomic orbitals of every included electronic shell. In Table 4 the SCF calculation results for energy components of cluster NiMn4Ga4 with various numbers of open shells with maximal value of total spin for ROHF and indefinite total spin for UHF calculations are presented. The similar results for DFT calculations are given in Table 5. Total energy for the last case is essentially larger then for the first one. This can be related to smaller basis set used for Ga atoms in DFT calculations. In Fig. 3 the histogram of energy spectrum of the cluster is presented. The spectrum was calculated by RHF method for singlet closed shall state and ROHF and UHF methods for triplet, quintet and septet open shell states. In NWChem package, ROHF method is realized in such a way that only state with definite maximal spin is calculated. This means that all

T. Breczko, V.V. Barkaline, R.M. Grechishkin, V.V. Nelayev62

electrons on single occupied shells have the same spin projection. For UHF method, term singlet is used for state with equal number of α- and β-electrons, triplet – for state with the number of α-electrons greater on 2 then that of β-electrons, quintet – for state with 4 excess α-electrons etc. Energy spectrum spin dependence for ROHF calculations is presented in Fig. 4, and it does not seem very strong. Table 3. Characteristics of basis sets.

Atom Atomic mass

Number of Gaussian functions

Type of Gaussian functions

Ni 57.935300 [Ar]3d84s2 6-31G** 12 39 5s4p2d1f Mn 54.938100 [Ar]3d54s2 6-31G** 12 39 5s4p2d1f Ga

68.925700 [Ar]3d104s24p1 6-311G** 18 47 8s7p3d 3-21G 10 24 5s4p1d

Table 4. SCF calculated energy data in hartrees.

Parameter Singlet Calcula- tion type

Triplet Quintet Septet

One-electron energy -28302.398

Two-electron energy 9948.029

ROHF 9945.288 9939.022 9938.927 UHF 9924.868 9931.702 9933.318

Nuclear repulsion energy 4557.270 all 4557.270 4557.270 4557.270 Table 5. DFT calculated energy data in hartrees.

Parameter Singlet Triplet Quintet Septet Total energy -13774.816 -13775.206 -13775.140 -13775.258 Coulomb energy 10495.345 10494.026 10494.696 10493.838 Exchange energy -573.100 -573.719 -573.618 -573.770 Nuclear repulsion energy 4557.270 4557.270 4557.270 4557.270

Fig. 3. Histogram of NiMn4Ga4 cluster energy spectrum with discretization 0.12 hartree. Common number of levels 383, RHF calculation. 126 molecular orbitals are double occupied. Highest occupied and lowest unoccupied molecular orbitals’ energies are inserted.

Magnetic properties of Ni2MnGa alloy 63

Fig. 4. Histogram of NiMnm4Ga4 cluster energy spectrum with discretization 0.026 hartree for various spin states from ROHF calculations near the HOMO and LUMO. Four neighbor lines correspond to the same interval. Isosurfaces of electron density of the cluster in singlet state both for SCF and DFT calculations are presented in Fig. 5. The difference between the results is associated with d- electrons of Mn atoms of the cluster. For highest spin states a ‘cubic’ form of density near Mn atoms is present only for ROHF calculation. For UHF and DFT methods the results are very close for a given spin state. It is interesting that the form of isosurfaces very slightly depends on the spin state of cluster. For triplet and quintet states they are very similar to those presented in Fig. 6 for septet state.

a) b) c)

d) e) f)

Fig. 5. Isosurfaces of electron density ρ for NiMn4Ga4 cluster in singlet state: a-c for RHF calculation, d-f for DFT calculation, a,d – isosurface corresponds to lg ρ=0; b,e – isosurface corresponds to lg ρ=-1.5; c,f - isosurface corresponds to lg ρ=-2.

Spin density studies show much less similarity of UHF and DFT calculations. For triplet state UHF calculation results in large spin density on Ga atoms which seems unseasonable. Clarifying this issue, one needs further investigation. Here we present only DFT results (Fig. 7). They show that Mn atoms play the main role in spin polarization of cluster and that this

T. Breczko, V.V. Barkaline, R.M. Grechishkin, V.V. Nelayev64

role is played by different Mn atoms in different manner. Ni atom reduces the total polarization of the cluster because its negative contribution relatively the general contribution of Mn atoms. But the last is reduced partially by the ‘clouds’ of the negative spin density around the regions of positive one. This complex behavior of spin polarization in NiMn4Ga4 cluster promises interesting results for Ni2MnGa cluster too. Such cluster of minimal size contains 35 atoms and for its study it is necessary to use supercomputer resources.

a) b) c)

d) e) f)

g) h) i) Fig. 6. Isosurfaces of electron density ρ for NiMm4Ga4 cluster in septet state: a-c for ROHF calculation, d-f for UHF calculation, g-i for DFT calculation a,d,g – isosurface corresponds to lg ρ=0; b,e,h – isosurface corresponds to lg ρ=-1.5 in atomic units; c,f,i - isosurface corresponds to lg ρ=-2.

Magnetic properties of Ni2MnGa alloy 65

a) b) c)

d) e) f)

g) h) i) Fig. 7. Isosurfaces of electron spin density ρS for NiMm4Ga4 cluster from DFT calculations: a-c for triplet state, d-f for quintet state, g-i for septet state; a,d,g – isosurface corresponds to lg|ρS|=0; b,e,h – isosurface corresponds to lg|ρS|=-1.5 in atomic units; c,f,i - isosurface corresponds to lg|ρS|=-2. 5. Conclusions The results obtained indicate that thermal stabilisation is important in stabilisation of martensitic structure. The incidental effect is there the appearance of microcracks along the interface. Properties of the system were investigated both experimentally and by ab initio simulation in NWChem package. Compatibility of Ni2MnGa crystal structure and cell parameters with semiconductors and also presence of spin-polarization of carriers opens up possibilities of the Ni2MnGa use in semiconductor spintronics. Acknowledgments The work was partially supported by EC FP7 project BalticGrid-II, grant 223807, Belarussian state program “Nanotech 2006-2010”, grant 4.19, and the “Triada” Scientific Technical Program of the Belarus-Russia Union State, grant 2.7. Authors want to express gratitude to EMSL for providing them with NWChem and ECCE packages. References

T. Breczko, V.V. Barkaline, R.M. Grechishkin, V.V. Nelayev66

[1] V.A. Chernenko, E. Cesari, V.V. Kokorin, I.N. Vitenko // Scripta Metallurgica et Materialia 33 (1995) 1239.

[2] V. Martynov, V. Kokorin // J. Phys. III (France) 2 (1996) 739. [3] T. Breczko, V. Nelayev, K. Dovzhik, M. Najbuk and M. Bramowicz // Proceedings of

NDTCS 13 (2008) 89. [4] A.A. Likhachev and K. Ullakko // Phys. Letters A275 (2000) 142. [5] Q. Pan and R.D. James // J. Appl. Phys. 87 (2000) 4702. [6] Y. Murakami, D. Shindo, K. Oikawa // Appl. Phys. Lett. 82 (2003) 3695. [7] Y. Kishi, C. Craciunescu, M. Sato, T. Okazaki, Y. Furuya, M. Wuttig // J. Magn. Magn.

Mater. 262 (2003) L186. [8] O.M. Korpusov, R.M. Grechishkin, V.V. Koledov, V.V. Khovailo, T. Takagi, V.G.

Shavrov, // J. Magn. Magn. Mater. 272-276 (2004) 2035. [9] V.A. Chernenko, A.R. Lopez, M. Kohl, M. Ohtsuka, I. Orue, J.M. Barandiaran // J. Phys.:

Condens. Matter 17 (2005) 5215. [10] T. Breczko, M. Bramowicz // Techn. Sci. No 7, 2004. [11] E.J. Bylaska, W.A. de Jong, N. Govind, K. Kowalski, T. P. Straatsma, M. Valiev, D.

Wang, E. Apra, T.L. Windus, J. Hammond, P. Nichols, S. Hirata, M.T. Hackler, Y. Zhao, P.-D. Fan, R.J. Harrison, M. Dupuis, D.M.A. Smith, J. Nieplocha, V. Tipparaju, M.Krishnan, Q. Wu, T. van Voorhis, A. A. Auer, M. Nooijen, E. Brown, G. Cisneros, G.I. Fann, H. Fruchtl, J. Garza, K. Hirao, R. Kendall, J.A. Nichols, K. Tsemekhman, K. Wolinski, J. Anchell, D. Bernholdt, P. Borowski, T.Clark, D. Clerc, H. Dachsel, M. Deegan, K.Dyall, D. Elwood, E. Glendening, M. Gutowski, A. Hess, J. Jaffe, B. Johnson, J. Ju, R. Kobayashi, R. Kutteh, Z. Lin, R.Littlefield, X. Long, B. Meng, T. Nakajima, S. Niu, L. Pollack, M. Rosing, G. Sandrone, M. Stave, H. Taylor, G. Thomas, J. van Lenthe, A. Wong, Z. Zhang, NWChem, A Computational Chemistry Package for Parallel Computers, Version 5.1. Richland, Washington 99352-0999: Pacific Northwest National Laboratory, 2007.

[12] T.M. Breczko, V. Nelayev, K. Dovzhik and M. Najbuk // Proc. of SPIE Vol.7377 (2008) 7377OK-19.

[13] H. Rumpf, C. Craciunescu, J. Feydt, A. Gilles1, M. Wuttig, E. Quandt, // Mat. Res. Soc. Symp.…

L rr σ from (13) can be represented as the product of spatial

orbital ),,,( 1 Mn RRr r

L rrψ and one of two spin functions )(σα or )(σβ corresponding to two

possible spin projection values of an electron. Expectation value of the electronic Hamiltonian eH N in LΦ state can be represented as

LL

( ) ,),,(),,( 2

1 ),,(),,(

r L

rr L

rr L

rr L

r (15)

where one-electron energies iE , Coulomb integrals ijJ and exchange integrals ijK all are

non-negative and defined as follows:

),,,,( 2

Obviously iiii KJ = .

Equations (16)-(18) show that for a fixed set of spin-orbitals contributing to

)RRr,r( MLLL

r L

rr L

r ,,,,,, 111 σσΦ the most adequate choose of the effective potential )(ri

r u

−= (19)

∑∫ ⋅ −

(21)

Such defined potential is named Hartree-Fock potential, it is non-local and depends on the spin-orbitals. The Koopman's theorem provides a physical interpretation of the orbital energies: it states that the orbital energy iε is an approximation of the ionization energy

associated with the removal of an electron from the orbital i .

Because of orbital dependence of Hartree-Fock potential, the orbitals themselves must be defined in a self-consistent manner. A trial set of spin-orbitals is formulated and used to

Magnetic properties of Ni2MnGa alloy 57

construct the Fock operator (11), where (18) is used for )(ri

r u , then the equations (12) are

solved to obtain a new set of spin-orbitals that are used to construct a revised Fock operator, and so on. The cycle of calculation and reformulation is repeated until a convergence criterion is satisfied. Such obtained spin-orbitals realize stationary point of energy (15) as functional of spin-orbitals (the latter are assumed to be orthonormal). In self-consistent field calculations on closed-shell states of atomic clusters with even number of electrons, it is supposed that the spatial parts of the spin-orbitals are identical for electrons of every electron pair. There are then L/2 spatial orbitals of the form

),,,( 1 Mn RRr r

.

)(),,,()(),,,(

)(),,,()(),,,(

)(),,,()(),,,(

)(),,,()(),,,(

rr

rrrr

(22)

.

)(),,,()(),,,(

)(),,,()(),,,(

)(),,,()(),,,(

)(),,,()(),,,(

)(),,,()(),,,(

rr

rrrr

(23)

In the unrestricted open-shell Hartree-Fock (UHF) formalism any two electrons are not constrained to the same spatial wave function and L-electron wave function has the general form (13). By relaxing the constraint of occupying orbitals in pairs, the open-shell UHF formalism gives a lower variational energy than the ROHF formalism. However, one disadvantage of the UHF approach is that whereas the RHF and ROHF wave functions are the eigenfunctions of the total cluster spin operator, the UHF function is not; that is, the total spin angular momentum is not well-defined for the UHF wavefunction. In practical calculations cluster spatial orbitals are expanded into a finite series of LK ≥

basis functions ),,( 1 Mk RRr r

L rrξ :

rr ξψ . (24)

It is useful to introduce vector and matrix notation for orbitals .}{};,,{};,,{ 11 kiKL C=== Cξψ ξξψψ LL (25)

Then, equation (24) can be rewritten as Cξψ = . (26)

T. Breczko, V.V. Barkaline, R.M. Grechishkin, V.V. Nelayev58

Then for closed shell RHF formalism energy relation (15) can be transformed to

,)} 2

r L

r (27)

If one introduces overlap matrix for the basis set orbitals

),,,(),,,( 11 MjMiij RRrRRrrd r

L rrr ξξ∫=S , the necessary and sufficient condition of

orthonormality for cluster orbitals can be represented as RRSR = . (31)

The stationarity condition for Hartree-Fock energy (27) accounting the orthonormality of the orbitals leads to Hartree-Fock matrix equations

SCεCGh =+ )( , (32) where ε is LL× matrix of Lagrange multipliers which can be chosen as a diagonal matrix with elements associated with the energies of corresponding cluster orbital. Similarly can be treated the case of open shells, with some sophistication of definition of G and C matrixes.

Density functional theory. An alternative to the HF methods is the density functional theory (DFT). DFT begins not with the multi-electron wavefunction

)RRr,r( MLL

r L

rr L

r ,,,,, 111 σσΦ and Schrödinger equation (7) but with the concept of the

electron probability density, which is defined as the integral over the spin coordinates of all electrons and over all but one of the spatial variables

)RRr,r()RRr,r(rdrdL

r

MLLMLLL

L

∑∫ ∫ (33)

This function determines the probability of finding any of the L electrons within a volume element rd

r . The reason for the popularity of DFT is that it takes into account electron

correlation. It can be used to do calculations on clusters of 100 or more atoms in significantly less time than HF methods. Integration of )(r

rρ over whole space gives the number of electrons in a cluster:

∫ = Lrrd )( rrρ . (34)

Major points of DFT theory is two Hohenberg-Kohn theorems. The first one demonstrates that the electron density uniquely determines the Hamiltonian operator and thus all the properties of the system. This theorem states that the external potential )(rN

r eV is (to

within a constant) a unique functional of )(r rρ . Since, in its turn )(rN

r eV fixes eH N , we see

Magnetic properties of Ni2MnGa alloy 59

that the full many particle ground state is a unique functional of )(r rρ . Thus, )(r

rρ

determines L and )(rN

r eV and hence all the properties of the ground state, for example the

kinetic energy ][ ρT , the potential energy of electron-nuclei interaction ][ ρeNV , the potential

energy of electron-electron interactions ][ ρeeV and the total electron energy ][ ρeNE , which

can be written as

,][)()(][][][][ ρρρρρρ HKNNN FrrrdVVTE +=++= ∫ rrr

eeeee V (35)

][][][ ρρρ eeVTFHK += . (36)

The second Hohenberg-Kohn theorem states that the functional ][ ρHKF , that delivers the ground state energy of the system, delivers the lowest energy if and only if the input density is the true ground state density. In other words this means that for any trial density )(~ r

rρ ,

which satisfies the necessary boundary conditions such as 0)(~ ≥r rρ , Lrrd =∫ )(~ rrρ , and

which is associated with some external potential )(rN

r eV , the energy obtained from functional

(35) represents an upper bound to the true ground state energy 0E . 0E results if and only if

the exact ground state density )(r rρ is inserted in (35).

From ][ ρeeV one can extract classical part ][ ρJ ,

][][][)()( 2

e rdrdV +=+

correction, exchange and Coulomb correlation. The explicit form of the functionals ][ ρT and ][ ρnclV is the major task of DFT. To relate

them to the well-known results of Hartree-Fock orbital theory the reference system of L non- interacting electrons with the same electron density function is introduced, for which the set of orthonormal spatial orbitals { } Liri ,,1,)( L

r =ψ defines

rhrr (39)

Then if one combines all unknown contributions into one energy term ][ ρXCE ,

,])[][(])[][(][ ρρρρρ JVTTE refXC −+−= ee (40)

the functional of cluster energy can be represented as

.][)()( 2 1

ee

(41)

The only term for which no explicit form can be given is ][ ρXCE . One now can apply the

variational principle to answer the question about what condition must the orbitals )(ri

rψ

fulfill in order to minimize the energy expression (41) under the usual constraint

ijji rrrd δψψ =∫ )()( rrr

,)()()( 2

ρ (43)

and δρρδ ][)( XCXC ErV =r is the variational derivative of exchange and correlation energy

functional. The value of )(rVKS

r depends on the density, and therefore the Kohn-Sham

equations have to be solved iteratively to obtain a self-consistent solution. Most of the applications of the Kohn-Sham density functional theory make use of the linear combination of atomic orbitals (LCAO) expansion of the Kohn-Sham orbitals. Similarly to (24), in this approach one introduces a set of K predefined basis functions

)(rk

∑ =

)()( rr ξψ . (44)

Basis functions for both SCF and DFT calculation usually are chosen among three possibilities:

I. Slater-type-orbitals (STO): they seem to be the natural choice for basis functions. They are exponential functions that mimic the exact eigenfunctions of a hydrogen atom. A typical STO is expressed as

),(1 θξ β lm

rnSTO YerN −−= . (45)

Here n corresponds to the principal quantum number, the orbital exponent is termed β and ),( θlmY are the usual spherical harmonics. Unfortunately, it is very difficult to

compute many-center integrals with STO basis, and they do not play a major role in ordinary quantum chemistry. II. Gaussian-type-orbitals (GTO). They have the following general form:

. 2rnmlGTO ezyxN αξ −= (46)

N is a normalization factor, α represents the orbital exponent. nmlJ ++= is used to classify the GTO as s-functions ( 0=J ), p-functions ( 1=J ), etc. III. Contracted Gaussian functions (CGF) basis sets, in which several Gaussian functions are combined in a fixed linear combination:

. 1

= = (47)

A variety of exchange-correlation functionals, having names such as mPWPW91, B3LYP, MPW1K, PBE1PBE, BLYP, BP91, and PBE, have been developed for use in DFT calculations; the names designate a particular pairing of an exchange functional and a correlation functional. For example, BLYP functional is a combination of the gradient- corrected exchange functional developed by A.D. Becke and the gradient-corrected correlation functional developed by C. Lee, W. Yang, and R.G. Parr. Some of the functionals, such as B3LYP, represent hybrid DFT calculations that use Hartree-Fock corrections in conjunction with density functional correlation and exchange Density functional theory has also been applied to study open-shell atoms and molecules on the basis of spin density concept. The spin density refers to the difference between the spin-up electron density and the spin-down electron density, and the exchange-correlation energy depends on the spin density as well as the total electron density. Namely such

Magnetic properties of Ni2MnGa alloy 61

approach has to be used in DFT investigations of the magnetic structures of metals and alloys. The original density functional theory has been generalized to deal with many different situations: spin polarized systems, multicomponent systems such as nuclei and electron hole droplets, free energy at finite temperatures, superconductors with electronic pairing mechanisms, relativistic electrons, time-dependent phenomena and excited states, bosons, molecular dynamics, etc. The computation time required for a DFT calculation formally scales as the third power of the number of basis functions; as a result, DFT methods are computationally more efficient (though not necessarily more accurate) than HF-based formalisms, which scale as the fourth power of the number of basis functions. 4. Computer simulations results and discussion Ni2MnGa Heusler alloys (HA) has a theoretical lattice constant of 5.811 Å (10.981 .u.) and 5.729 Å (10.826 .u.) for the ferromagnetic and the paramagnetic phase, respectively. The crystal structure of Ni2MnGa HA can be considered as a bcc-based fcc crystal with a chain of Ni-Mn-Ni-Ga along the <111> direction. In present paper simulations deal with the simplest structure unit of the material – the cluster containing 9 atoms which is presented in Fig. 2. We calculate electronic structure of this cluster by open shell restricted Hartree-Fock method (ROHF), by unrestricted Hartree-Fock method and density functional theory (DFT) using NWChem package [11]1. All calculations deal with the system of 252 electrons.

Fig. 2. Atomic structure of cluster NiMn4Ga4, the constitutive element of L21 cubic form of

Ni2MnGa. Basis sets used in calculations are presented in Table 3. In all cases 6-31G* was used to represent atomic orbitals of Ni and Mn, and 6-311G** for Ga atoms in ROHF calculations. For DFT calculations the simplest 3-21G basis set for Ga was used. Contracted Gaussian functions (47) are used to represent atomic orbitals of every included electronic shell. In Table 4 the SCF calculation results for energy components of cluster NiMn4Ga4 with various numbers of open shells with maximal value of total spin for ROHF and indefinite total spin for UHF calculations are presented. The similar results for DFT calculations are given in Table 5. Total energy for the last case is essentially larger then for the first one. This can be related to smaller basis set used for Ga atoms in DFT calculations. In Fig. 3 the histogram of energy spectrum of the cluster is presented. The spectrum was calculated by RHF method for singlet closed shall state and ROHF and UHF methods for triplet, quintet and septet open shell states. In NWChem package, ROHF method is realized in such a way that only state with definite maximal spin is calculated. This means that all

T. Breczko, V.V. Barkaline, R.M. Grechishkin, V.V. Nelayev62

electrons on single occupied shells have the same spin projection. For UHF method, term singlet is used for state with equal number of α- and β-electrons, triplet – for state with the number of α-electrons greater on 2 then that of β-electrons, quintet – for state with 4 excess α-electrons etc. Energy spectrum spin dependence for ROHF calculations is presented in Fig. 4, and it does not seem very strong. Table 3. Characteristics of basis sets.

Atom Atomic mass

Number of Gaussian functions

Type of Gaussian functions

Ni 57.935300 [Ar]3d84s2 6-31G** 12 39 5s4p2d1f Mn 54.938100 [Ar]3d54s2 6-31G** 12 39 5s4p2d1f Ga

68.925700 [Ar]3d104s24p1 6-311G** 18 47 8s7p3d 3-21G 10 24 5s4p1d

Table 4. SCF calculated energy data in hartrees.

Parameter Singlet Calcula- tion type

Triplet Quintet Septet

One-electron energy -28302.398

Two-electron energy 9948.029

ROHF 9945.288 9939.022 9938.927 UHF 9924.868 9931.702 9933.318

Nuclear repulsion energy 4557.270 all 4557.270 4557.270 4557.270 Table 5. DFT calculated energy data in hartrees.

Parameter Singlet Triplet Quintet Septet Total energy -13774.816 -13775.206 -13775.140 -13775.258 Coulomb energy 10495.345 10494.026 10494.696 10493.838 Exchange energy -573.100 -573.719 -573.618 -573.770 Nuclear repulsion energy 4557.270 4557.270 4557.270 4557.270

Fig. 3. Histogram of NiMn4Ga4 cluster energy spectrum with discretization 0.12 hartree. Common number of levels 383, RHF calculation. 126 molecular orbitals are double occupied. Highest occupied and lowest unoccupied molecular orbitals’ energies are inserted.

Magnetic properties of Ni2MnGa alloy 63

Fig. 4. Histogram of NiMnm4Ga4 cluster energy spectrum with discretization 0.026 hartree for various spin states from ROHF calculations near the HOMO and LUMO. Four neighbor lines correspond to the same interval. Isosurfaces of electron density of the cluster in singlet state both for SCF and DFT calculations are presented in Fig. 5. The difference between the results is associated with d- electrons of Mn atoms of the cluster. For highest spin states a ‘cubic’ form of density near Mn atoms is present only for ROHF calculation. For UHF and DFT methods the results are very close for a given spin state. It is interesting that the form of isosurfaces very slightly depends on the spin state of cluster. For triplet and quintet states they are very similar to those presented in Fig. 6 for septet state.

a) b) c)

d) e) f)

Fig. 5. Isosurfaces of electron density ρ for NiMn4Ga4 cluster in singlet state: a-c for RHF calculation, d-f for DFT calculation, a,d – isosurface corresponds to lg ρ=0; b,e – isosurface corresponds to lg ρ=-1.5; c,f - isosurface corresponds to lg ρ=-2.

Spin density studies show much less similarity of UHF and DFT calculations. For triplet state UHF calculation results in large spin density on Ga atoms which seems unseasonable. Clarifying this issue, one needs further investigation. Here we present only DFT results (Fig. 7). They show that Mn atoms play the main role in spin polarization of cluster and that this

T. Breczko, V.V. Barkaline, R.M. Grechishkin, V.V. Nelayev64

role is played by different Mn atoms in different manner. Ni atom reduces the total polarization of the cluster because its negative contribution relatively the general contribution of Mn atoms. But the last is reduced partially by the ‘clouds’ of the negative spin density around the regions of positive one. This complex behavior of spin polarization in NiMn4Ga4 cluster promises interesting results for Ni2MnGa cluster too. Such cluster of minimal size contains 35 atoms and for its study it is necessary to use supercomputer resources.

a) b) c)

d) e) f)

g) h) i) Fig. 6. Isosurfaces of electron density ρ for NiMm4Ga4 cluster in septet state: a-c for ROHF calculation, d-f for UHF calculation, g-i for DFT calculation a,d,g – isosurface corresponds to lg ρ=0; b,e,h – isosurface corresponds to lg ρ=-1.5 in atomic units; c,f,i - isosurface corresponds to lg ρ=-2.

Magnetic properties of Ni2MnGa alloy 65

a) b) c)

d) e) f)

g) h) i) Fig. 7. Isosurfaces of electron spin density ρS for NiMm4Ga4 cluster from DFT calculations: a-c for triplet state, d-f for quintet state, g-i for septet state; a,d,g – isosurface corresponds to lg|ρS|=0; b,e,h – isosurface corresponds to lg|ρS|=-1.5 in atomic units; c,f,i - isosurface corresponds to lg|ρS|=-2. 5. Conclusions The results obtained indicate that thermal stabilisation is important in stabilisation of martensitic structure. The incidental effect is there the appearance of microcracks along the interface. Properties of the system were investigated both experimentally and by ab initio simulation in NWChem package. Compatibility of Ni2MnGa crystal structure and cell parameters with semiconductors and also presence of spin-polarization of carriers opens up possibilities of the Ni2MnGa use in semiconductor spintronics. Acknowledgments The work was partially supported by EC FP7 project BalticGrid-II, grant 223807, Belarussian state program “Nanotech 2006-2010”, grant 4.19, and the “Triada” Scientific Technical Program of the Belarus-Russia Union State, grant 2.7. Authors want to express gratitude to EMSL for providing them with NWChem and ECCE packages. References

T. Breczko, V.V. Barkaline, R.M. Grechishkin, V.V. Nelayev66

[1] V.A. Chernenko, E. Cesari, V.V. Kokorin, I.N. Vitenko // Scripta Metallurgica et Materialia 33 (1995) 1239.

[2] V. Martynov, V. Kokorin // J. Phys. III (France) 2 (1996) 739. [3] T. Breczko, V. Nelayev, K. Dovzhik, M. Najbuk and M. Bramowicz // Proceedings of

NDTCS 13 (2008) 89. [4] A.A. Likhachev and K. Ullakko // Phys. Letters A275 (2000) 142. [5] Q. Pan and R.D. James // J. Appl. Phys. 87 (2000) 4702. [6] Y. Murakami, D. Shindo, K. Oikawa // Appl. Phys. Lett. 82 (2003) 3695. [7] Y. Kishi, C. Craciunescu, M. Sato, T. Okazaki, Y. Furuya, M. Wuttig // J. Magn. Magn.

Mater. 262 (2003) L186. [8] O.M. Korpusov, R.M. Grechishkin, V.V. Koledov, V.V. Khovailo, T. Takagi, V.G.

Shavrov, // J. Magn. Magn. Mater. 272-276 (2004) 2035. [9] V.A. Chernenko, A.R. Lopez, M. Kohl, M. Ohtsuka, I. Orue, J.M. Barandiaran // J. Phys.:

Condens. Matter 17 (2005) 5215. [10] T. Breczko, M. Bramowicz // Techn. Sci. No 7, 2004. [11] E.J. Bylaska, W.A. de Jong, N. Govind, K. Kowalski, T. P. Straatsma, M. Valiev, D.

Wang, E. Apra, T.L. Windus, J. Hammond, P. Nichols, S. Hirata, M.T. Hackler, Y. Zhao, P.-D. Fan, R.J. Harrison, M. Dupuis, D.M.A. Smith, J. Nieplocha, V. Tipparaju, M.Krishnan, Q. Wu, T. van Voorhis, A. A. Auer, M. Nooijen, E. Brown, G. Cisneros, G.I. Fann, H. Fruchtl, J. Garza, K. Hirao, R. Kendall, J.A. Nichols, K. Tsemekhman, K. Wolinski, J. Anchell, D. Bernholdt, P. Borowski, T.Clark, D. Clerc, H. Dachsel, M. Deegan, K.Dyall, D. Elwood, E. Glendening, M. Gutowski, A. Hess, J. Jaffe, B. Johnson, J. Ju, R. Kobayashi, R. Kutteh, Z. Lin, R.Littlefield, X. Long, B. Meng, T. Nakajima, S. Niu, L. Pollack, M. Rosing, G. Sandrone, M. Stave, H. Taylor, G. Thomas, J. van Lenthe, A. Wong, Z. Zhang, NWChem, A Computational Chemistry Package for Parallel Computers, Version 5.1. Richland, Washington 99352-0999: Pacific Northwest National Laboratory, 2007.

[12] T.M. Breczko, V. Nelayev, K. Dovzhik and M. Najbuk // Proc. of SPIE Vol.7377 (2008) 7377OK-19.

[13] H. Rumpf, C. Craciunescu, J. Feydt, A. Gilles1, M. Wuttig, E. Quandt, // Mat. Res. Soc. Symp.…